* Abstract—*The effect of thermally induced stress on the modal
properties of highly elliptical core optical fibers is studied in this
work using a finite element method. The stress analysis is carried out
and anisotropic refractive index change is calculated using both the
conventional plane strain approximation and the generalized plane
strain approach. After considering the stress optical effect, the modal
analysis of the fiber is performed to obtain the solutions of
fundamental and higher order modes. The modal effective index,
modal birefringence, group effective index, group birefringence, and
dispersion of different modes of the fiber are presented. For
propagation properties, it can be seen that the results depend much on
the approach of stress analysis.

* Keywords—*Birefringence, dispersion, elliptical core fiber,
optical mode analysis, stress-optic effect, stress analysis.

I. INTRODUCTION

OLARIZATION maintaining fibers (PMF) have been widely
used for polarization control in fiber optic sensors,
precision optical instruments, and optical communication
systems [1]-[5]. Different structured fibers like bow-tie fibers,
PANDA fibers, side-pit fibers, side-tunnel fibers have been
analyzed to show different propagation properties previously
[3]-[9]. These types of fibers are designed to introduce a
differential stress in the core so that the state of polarization of
the guided light wave can be maintained by means of
stress-optic effect [3]-[9]. Another fiber is designed to have an
asymmetric core shape, *i*.*e*., elliptical core to introduce
birefringence in order to maintain the polarization [1]-[11].

In the elliptical core fibers, the birefringence primarily originated from the core ellipticity. But, like the other fibers, there is temperature induced birefringence also. Both the effects should be considered very carefully to find the accurate modal characteristics. In many cases, they have been considered, but only for fundamental modes [1]-[5], [7], [10]-[14]. In [10]-[11], modal analysis is carried out for fundamental and higher order modes, but stress effects have not been considered. As for analysis methods, many different approaches are used for analyzing PMFs [6]-[16]. Among them the finite element method (FEM) is suitable for producing accurate modal solutions of different types of fibers [10]-[11], [13], [17], though there are different approaches

M. Shah Alam and Sarkar Rahat M. Anwar are with the Department of Electrical and Electronic Engineering, Bangladesh University of Engineering and Technology (BUET), Dhaka-1000, Bangladesh (corresponding author phone: +880-2-9665650 ext- 7279; e-mail: shalam@ eee.buet.ac.bd).

with this method. Very recently, the authors have reported modal solutions of fundamental and higher order modes of highly elliptical core fibers considering plane strain approach to incorporate stress-optic effects in the analysis [18], where only the dependence of birefringence properties with core ellipticity is discussed and field distributions of different modes are shown.

In this work, the structure with highly elliptical core optical
fiber with a circular cladding is analyzed by using the FEM
[17] to show the effects of the approach of stress analysis on
modal characteristics. The plane strain approximation and also
the generalized plane strain approach have been considered
here to include the stress-optic effect and the results of
propagation characteristics are compared to show the
influences of stress analysis approach on optical analysis.
After considering the stress-optic effect, an optical mode
solver with the electric field as the working variable is
employed to obtain the modal solutions. Thus, the effects of
thermally induced stress on the fundamental and higher order
modes of highly elliptical core optical fibers are studied. It
has been seen that higher ellipticity of the core results much
higher thermal stress in the fiber core, which in turn produces
higher birefringence to produce non-degenerate modes in the
fiber. Also, for propagation properties, the results depend
much on the approach of stress analysis.** **

II. THEORY

A high value of birefringence is usually desired for single mode operation in an optical fiber. During the manufacturing process, due to different thermal expansion coefficients of core and cladding material, the fiber becomes stressed. This stress causes the indices to become anisotropic and increases the birefringence of orthogonal polarized wave in the fiber. Along with this thermally induced birefringence, there can be geometrical birefringence, which is usually achieved by making the core a non-circular one [19]. For predicting light propagation performance of a fiber, both the geometrical and thermal induced birefringence effects have to be considered in the analysis [20].

To understand the overall birefringence of a fiber with elliptical core, it is necessary to carry out the stress analysis first to find the stress distribution and hence the change in refractive index due to stress-optic effect. Next, the optical analysis is to be performed with the new refractive index to obtain the modal solutions, birefringence, and propagation

### Modal Propagation Properties of Elliptical Core

### Optical Fibers Considering Stress-Optic Effects

### M. Shah Alam and Sarkar Rahat M. Anwar

## P

properties. In this work, the stress analysis has been carried out using two approaches and the difference in numerical results of the propagation properties have been studied.

*A.* *Stress Analysis *

The effect of thermally induced stress on the refractive index in different domains in the cross section of the fiber can be determined using generalized plane strain approach or the plane strain approximation [17]. The generalized plane strain approach differs from the plane strain approximation in that the longitudinal strain is no longer zero in the generalized plane strain approach. Also, the strain is linearly varying over the cross section of the fiber in generalized approach. The system formulation is carried out for unknown displacements due to strain over the cross section of the fiber. After solving the system for unknown displacements, one can easily obtain the stresses σx, σy, and σz and can find the anisotropic change

in refractive indices due to stress-optic effect. The new refractive indices are given by

0 2 1
0 2 1
0 2 1
( )
( )
( )
*x* *x* *y* *z*
*y* *y* *z* *x*
*z* *z* *x* *y*
*n* *n* *C* *C*
*n* *n* *C* *C*
*n* *n* *C* *C*

### σ

### σ

### σ

### σ

### σ

### σ

### σ

### σ

### σ

= − − + = − − + = − − + . (1)Here *C*1 and *C*2 are the stress-optic coefficients and *n*0 is the

isotropic refractive index of the unstressed fiber material. The

*n*x, *n*y, and *n*z are the principal diagonal components of

anisotropic refractive index tensor when the stress-optic effect is incorporated. The refractive index of unstressed fiber material at different wavelengths may be obtained using Sellmeier equation [6].

*B.* *Optical Analysis *

In the optical analysis, the resulting anisotropic refractive
indices as calculated by (1) are used. The modal analysis is
carried out assuming that the wave propagates along the *z*
-direction and the electric field of the wave has the form [17]

### ( , , , )

*x y z t*

### =

### ( , ) exp[ (

*x y*

*j t*

### ω

### −

### β

*z*

### )]

**E**

**E**

, (2)
where ω is the angular frequency and β is the propagation constant. An eigenvalue equation in terms of the electric field can be obtained from the Helmholtz equation

2 2

0

### (

*n*

− ### )

*k*

### ∇ ×

### ∇ ×

**E**

### −

**E**

### =

**0**

, (3)
and is solved for modal effective index, *n*eff =

*β*/

*k*0, as the

eigenvalue. The boundary condition for electric field at the outside of the cladding boundary was set to zero. In [17], however, a module based on the perpendicular hybrid mode wave using transversal fields is used for finding the modal solutions.

III. RESULTS AND DISCUSSION

The cross section of the optical fiber with elliptical core is
shown in Fig. 1, where the core dimensions in *x*-direction
(major axis) and *y*-direction (minor axis) are 2*a* and 2*b*,
respectively. The cladding is circular with radius, *r*=25µm.
The refractive indices of core and cladding are *n*1 and *n*2,

respectively. The cross section of the fiber is meshed with

quadratic triangular elements in both stress analysis and
optical analysis. For stress analysis, the boundary conditions
are taken in such a way that along *x*-axis through the center of
the core, no displacement is allowed in *y*-direction, and along

*y*-axis through the center of the core, no displacement is
allowed in *x*-direction, and in other regions, no restrictions are
applied.

The values taken for stress-optic coefficients are

*C*1=4.184×10−12m2/N and *C*2=7.5714×10−13m2/N. The thermal

expansion coefficients of core and cladding are,

*α*core=2×10−6K−1 and *α*clad=1×10−6K−1. The Young’s modulus

of the fiber core and cladding material, *E*=72.324×109Pa and
the Poisson’s ratio, υ=0.186. The initial temperature of the
fiber is 1020°C and the final temperature when the fiber is
cooled down is 20°C. So, the temperature difference is
1000°C, which causes the thermal strain over the fiber cross
section. As the core is not circular and have different thermal
expansion coefficient than the cladding, the stress distribution
will not be equal in all the directions.

2*a*
2*b*
Cladding
Core
*x*
*y*
2*a*
2*b*
Cladding
Core
*x*
*y*

Fig. 1: Cross section of the optical fiber with elliptical core.

### (a) (b)

Fig. 2: (a) Vector displacement, and (b) Stress distribution, over the cross section of the fiber.

Fig. 2 shows the vector displacement due to deformation caused by strain in the fiber and stress distribution over the cross section of the fiber that occur because of different thermal expansion coefficients. The length of the arrow in Fig. 2(a) is proportional to the amount of displacement and the direction of the arrow is the direction of the displacement. It can be seen easily that the displacement is towards the center

of the fiber and lateral contraction occurs. From Fig. 2(b), it
can be seen that the stress is more at the core than at the
cladding region. This is expected as the displacement is
towards the center, more stress develops at the center of the
fiber. Here *a*=11.67µm, *b*=5µm, and ellipticity, ξ=0.4 are
taken throughout the calculation and the ellipticity is defined
by
( )
( )
*a b*
*a b*
ξ= −
+ .

Due to the stress-optic effect, the refractive index of both
core and cladding changes. This is shown for *n*x in Fig. 3.

With the development of stress, it can be seen that in the core
and cladding regions, the refractive index is decreased and at
the interface of core and cladding, it decreases abruptly.
However, the changed value depends on the associated stress
analysis technique. With the plane strain approach, the new
value of the index is much lowered than that given by
generalized plane strain approach. It can be seen that in the
core region, the refractive index, *n*x, is decreased from

1.46552 to 1.4652 for generalized plane strain and to 1.46514
for plane strain approximation, while in the cladding region,
for generalized plane strain, the refractive index shows a
minimum value of 1.44384 at the interface of core and
cladding, it increases towards the edge of the fiber to 1.44404,
which is greater than the original value of 1.44402. But when
the plane strain approximation is used, *n*x increases from

1.44378, at the interface to 1.44398, at the edge of the fiber to 1.44402, which

(a)

(b) (c)

Fig. 3: Variation of refractive index along *x*-axis, (a) in the fiber from
center of the core to the cladding boundary, (b) in the core region, (c)

in the cladding region.

(a) (b) (c) (d) (e) (f)

Fig. 4: Electric field intensity distribution of different modes of the fiber, (a) HEy11, (b) HEx11, (c)TE01, (d) TM01, (e) HEy12, (f) HEx12. is less than the original value. May be this is the reason why the optical characteristics of the fiber varies with the

associated stress analysis technique.

The anisotropic change in refractive index due to
stress-optic effect will cause a higher value of birefringence in the
fiber and the birefringence will cause the fundamental and
higher order modes to split, which are usually two-fold
degenerate modes in unstressed fiber. The electric field
intensity distribution of different modes over the cross section
of the fiber are shown in Fig. 4. In Fig. 4, fundamental and
higher order modal solutions are shown, where part (a) and (b)
show *y*-polarized and *x*-polarized fundamental HE11 modes,

respectively, part (c) and (d) show *y*-polarized TE01 mode and
*x*-polarized TM01 modes, respectively, part (e) and (f) show *y*

-polarized HE12 mode and *x*-polarized HE12 modes,

respectively.

Next, in Fig. 5, the dominant electric field intensity of the
fibers for thermally stressed condition and unstressed
condition are shown for different modes. The electric field
value is taken over the radial line along the *x*-axis from the
center of the fiber. From these curves, it can be seen that for
all the modes considered here, the field intensity distribution
remain similar in all the three cases of analysis.

(a) (b)

(c) (d)

(e) (f)

Fig. 5: Electric field intensity over the radial distance along *x*-axis,
(a) HEx11, (b) HEy11 , (c) TE01, (d) TM01, (e) HEx12,

and (f) HEy12 mode.

The birefringence of optical fiber for fundamental and higher order modes are shown as a function of wavelength in

Fig. 6. Part (a), (b), and (c) of this figure show the
birefringence of fundamental HE modes, TE-TM modes, and
higher order HE modes, designated by *B*11, *B*01, and *B*12,

respectively. The solid lines and dashed lines show the birefringence when the modal optical analysis incorporates indices of plane strain approach and generalized plane strain approach, respectively. The dotted line shows the birefringence when no thermal stress is considered. Birefringence differs much when thermal stress in the fiber is

(a)

(b)

(c)

Fig. 6: Variation of Birefringence with wavelength, (a) B11, (b) B01, and (c) B12.

Fig. 7: Variation of Birefringence with wavelength (extracted results from Fig. 6).

considered. Also, the approach of stress analysis to incorporate the stress-optic effect plays a vital role to obtain the predicted value of the birefringence. The difference in the results of plane strain based analysis and generalized plane strain based analysis is about 8-10% for all birefringences over the spectrum considered here. The generalized plane strain based analysis, however, gives higher values.

Most importantly, the numerical results show that the value of birefringence is improved by at least one decimal place when thermal stress induced changes in material index is incorporated. As in reality, the thermal stress induced effect is always there in the fiber material, any sort of modeling must incorporate the stress-optic effect. Without considering the effect may lead to erroneous prediction of performance. Now, it can also be seen that the birefringence increases slightly with the increase in wavelength and this is shown in Fig. 7. These results are the extracted values from Fig. 6 when generalized plane strain is considered for incorporating the stress-optic effect. In this figure, the dotted, dashed, and solid lines are showing the birefringence values for fundamental HE modes, TE-TM modes, and higher order HE modes, respectively.

Next, considering the stress-optic effect using generalized plane strain, the wavelength dependence of other propagation properties, e.g., beat length, chromatic dispersion, group birefringence, and group effective index of different modes are studied. Fig. 8 shows the variation of beat length with wavelength. The solid line, dashed line, and dotted line show beat lengths for fundamental HE modes, transverse modes, higher order HE modes, respectively. For all the three cases, beat length increases linearly with the increase in wavelength. Here the beat lengths are obtained from the phase birefringence of the respective modes.

In Fig. 9, the dependence of group effective indices of different modes with wavelength is shown. It is interesting to see that the group effective indices increase with the increase in the wavelength. The rate of increase or the slope of the curve is larger for higher order modes than the immediate

lower order modes. A clear difference can be seen in the group index of orthogonal pairs of modes over the wavelength range considered here.

In Fig. 10, the change of group birefringence with wavelength is shown for fundamental and higher order modes. In this figure, the solid line, dashed line, and the dotted line are showing the group birefringence values for fundamental HE modes, TE-TM modes, and higher order HE modes, respectively. It can be seen that the value of group birefringence of all the modes considered here increases with the increase of wavelength and the values are in the order of 10−4. Finally, Fig. 11 shows group velocity dispersion versus wavelength of different modes. The dispersion curves show that they are polarization independent and show increasing tendency with the increase in wavelength.

Fig. 8: Variation of Beat Length with wavelength.

Fig. 9: Group effective index versus wavelength.

Fig. 10: Variation of Group Birefringence with wavelength.

Fig. 11: Variation of group velocity dispersion with wavelength for different modes.

IV. CONCLUSION

The effect of thermally induced stress on fundamental and higher order modes of a highly elliptical core optical fiber is studied in this work. The birefringence of different modes show lower values when the modal analysis is carried out without considering thermal stress in the fiber. The stress developed in a fiber during manufacturing process, causes higher values of birefringence of fundamental and higher order modes of the fiber. However, the computation of modal birefringence and other propagation properties depend much on the approach of associated stress analysis. Also, it has been found that the birefringence and the dispersion of fundamental and higher order modes increase with an increase in the wavelength.

REFERENCES

[1] W. Urbanczyk, T. Martynkien, and W. J. Bock, “Dispersion effects in elliptical-core highly birefringent fibers,” Appl. Optics., vol. 40, no. 12, pp. 1911-1920, April 2001.

[2] I. –K. Hwang, Y. –H. Lee, K. Oh, and D. N. Payne, “High birefringence in elliptical hollow optical fiber,” Optics Express, vol. 12, no. 9, pp. 1916-1923, May 2004.

[3] J. Noda, K. Okamoto, and Y. Sasaki, “Polarization-Maintaining Fibers and Their Applications,” IEEE J. Lightwave Technol., vol. LT-4. no. 8, pp. 1071-1089, Aug. 1986.

[4] Y. Liu, B.M.A. Rahman, and K.T.V. Grattan, “Analysis of the Birefringence Properties of Optical Fibers Made by a Preform Deformation Technique,” IEEE J. Lightwave Technol., vol. 13, no. 2, pp. 142-147, Feb. 1995.

[5] Y. Liu, B. M. A Rahman, and K.T.V. Grattan, “Thermal-stress-induced birefringence in bow-tie optical fibers,” Appl. Optics, vol. 33, no. 24, pp. 5611-5616, Aug. 1994.

[6] K. Okamoto, Fundamentals of Optical Waveguides, Academic Press, 2000.

[7] K. Okamoto, T. Hosaka, and T. Edahiro, “Stress analysis of optical fibers by a finite element method,” IEEE J. Quantum Electron., vol. QE-17, pp. 2123-2129, Oct. 1981.

[8] M. Fontaine, “Computations of optical birefringence characteristics of highly eccentric elliptical core fibers under various thermal stress conditions,” J. Appl. Phys., vol. 75, no. 1, pp. 68-73, Jan. 1994. [9] M. Fontaine, B. Wu, V. P. Tzolov, W. J. Bock, and W. Urbanczyk,

“Theoretical and Experimental Analysis of Thermal Stress Effects on Modal Polarization Properties of Highly Birefringent Optical Fibers,” IEEE J. Lightwave Technol., vol. 14, no. 4, pp. 585-591, Apr. 1996.

[10] M. Eguchi and M. Koshiba, “Accurate Finite-Element Analysis of Dual-Mode Highly Elliptical-Core Fibers,” IEEE J. Lightwave Technol., vol. 12. no. 4, pp. 607-613, Apr. 1994.

[11] M. Eguchi and M. Koshiba, “Behavior of the First Higher-Order Modes of a Circular Core Optical Fiber Whose Core Cross-Section Changes into an Ellipse,” IEEE J. Lightwave Technol., vol. 13. no. 2, pp. 127-136, Feb. 1995.

[12] T. Schreiber, H. Schultz, O. Schmidt, F. Roser, J. Limpert, and A. Tunnermann, “Stress-induced birefringence in large-mode-area micro-structured optical fibers,” Optics Express, vol. 13, no. 10, pp. 3637-3645, May 2005.

[13] M. S. Alam, N. Somasiri, B. M. A. Rahman, and K. T. V. Grattan, “Effects of High External Pressure on Photonic Crystal Fiber,” Proceedings of the Third International Conference on Electrical and Computer Engineering, ICECE 2004, Dhaka, Bangladesh, pp. 245-248, Dec. 2004.

[14] Y. Jung, S. R. Han, S. Kim, U. C. Paek, and K. Oh, “Versatile control of geometric birefringence in elliptical hollow optical fiber,” Optics Lett., vol. 31, no. 18, pp. 2681-2683, Sept. 2006.

[15] H. Shu and M. Bass, “Calculating the Guided Modes in Optical Fibers and Waveguides,” IEEE J. Lightwave Technol., vol. 25, no. 9, pp. 2693-2699, Sept. 2007.

[16] Y. Zhu, X. Chen, Y. Xu, and Y. Xia, “Propagation Properties of Single-Mode Liquid-Core Optical Fibers With Subwavelength Diameter,” IEEE J. Lightwave Technol., vol. 25, no. 10, pp. 3051-3056, Oct. 2007. [17] COMSOL Multiphysics, version 3.2, Sept. 2005.

[18] R. M. Anwar and M. S. Alam, “Thermal Stress Effects on Higher Order Modes in Highly Elliptical Core Optical Fibers,” Proceedings of the Fifth International Conference on Electrical and Computer Engineering, ICECE 2008, pp. 561-565 , Dhaka, Bangladesh, Dec. 2008.

[19] D. A. Nolan, G. E. Berkey, M. –J. Li, X. Chen, W. A. Wood, and L. A. Zenteno, “Single-polarization fiber with a high extinction ratio,” Optics Lett., vol. 29, no. 16, pp. 1855-1857, Aug. 2004.

[20] E. M. Dianov and V. M. Mashinsky, “Germania-Based Core Fibers,” IEEE J. Lightwave Technol., vol. 23, no. 11, pp. 3500-3508, Nov. 2005.

**M. Shah Alam** (M’97-SM’04) received the B.Sc. Eng.,
M.Sc. Eng., and the Ph.D. degrees in Electrical and
Electronic Engineering in 1989, 1994, and 1997,
respectively. He was awarded a gold medal for outstanding
performance in B.Sc. Engineering examination. He received
the Japanese Government Scholarship from April 1991 to
March 1997 for pursuing his graduate studies, and received his Ph.D. degree
from Hokkaido University, Sapporo, Japan.

In 1997, he was a visiting researcher in Electrotechnical Laboratory, Tsukuba, Japan. Then in 1998, he became a lecturer in the Department of Electrical and Electronic Engineering, Bangladesh University of Engineering and Technology (BUET), Dhaka, Bangladesh, where he is now an Associate Professor. From Aug. 2003 to June 2004, he was on postdoctoral study leave from BUET and worked as a research fellow with the photonics research group in City University London, UK. His current research interests include optical fibers, photonic crystal fibers, amplification properties in fibers, electrooptic modulators, and the application of numerical techniques to integrated photonics problems and microwave integrated circuits.

Dr. Alam is a member of Bangladesh Computer Society and the Institution of Engineers, Bangladesh.

**Sarkar Rahat M. Anwar** received his B.Sc. Eng. Degree in Electrical and
Electronic Engineering from Bangladesh University of Engineering and
Technology (BUET), Dhaka, Bangladesh in 2008.